4 Argillaceous Rocks (CaCO3 < 40%) ClaysShalesSlatesPortland cement is made by mixing substances containing CaCO3 with substances containing SiO2, Al2O3, Fe2O3 and heating them to a clinker which is subsequently ground to powder and mixed with 2-6 % gypsum.
6 PRODUCTION STEPS Raw materials are crushed, screemed & stockpiled. Raw materials are mixed with definite proportions to obtain “raw mix”. They are mixed either dry (dry mixing) or by water (wet mixing).Prepared raw mix is fed into the rotary kiln.As the materials pass through the kiln their temperature is rised upto °C. The process of heating is named as “burning”. The output is known as “clinker” which is cm in diameter.
7 Clinker is cooled & stored. Clinker is ground with gypsum (3-6%) to adjust setting time.Packing & marketting.
11 REACTIONS IN THE KILN ~100°C→ free water evaporates. ~ C°→ loosely bound water is lost from clay.~ °C→decomposition of clay→SiO2&Al2O3~600°C→decomposition of MgCO3→MgO&CO2 (evaporates)~900°C→decomposition of CaCO3→CaO&CO2 (evaporates)
12 ~1250-1280°C→liquid formation & start of compound formation. ~1280°C→clinkering begins.~ °C→clinkering~100°C→clinker leaves the kiln & falls into a cooler.Sometimes the burning process of raw materials is performed in two stages: preheating upto 900°C & rotary kiln
13 CHEMICAL COMPOSITION OF P.C. Portland cement is composed of four major oxides (CaO, SiO2, Al2O3, Fe2O3 ≥90%) & some minor oxides. Minor refers to the quantity not importance.
14 SO3→from gypsum→not from the clinker OxideCommon NameAbbreviationApprox. Amount (%)CaOLimeC60-67SiO2SilicaS17-25Al2O3AluminaA3-8Fe2O3Iron-oxideF0.5-6MgOMagnesiaM0.1-4Na2OSodaNK2OPotassaKSO3Sulfuric AnhydrideŚ1-3CaO→limestoneSiO2-Al2O3→ClayFe2O3→Impurity in ClaysSO3→from gypsum→not from the clinker
15 A typical analysis of O.P.C. The amount of oxides in a P.C. Depend on the proportioning of the raw materials and how well the burning is done in the kiln. The chemical composition is found by chemical analysis.A typical analysis of O.P.C.Insoluble residue=0.2Loss on ignition=1.4C63.6S20.7A6F2.4Ś2.1M2.6N0.1K0.9Free C1.4Total99.8
16 CaO (C), SiO2 (S), Al2O3 (A) & Fe2O3 are the major oxides that interact in the kiln & form the major compounds.The proportions of these oxides determine the proportions of the compounds which affect the performance of the cement.SO3→comes largely from gypsumP.C. alone sets quickly so some gypsum is ground with clinker to retard the setting time.
17 If too much gypsum is included it leads to distruptive expansions of the hardened paste or concrete. ASTM C 150 → SO3 ≤ 3% in O.P.C.MgO+H2O→MHC+H→CH volume expansion & cause cracking.ASTM C 150 → M<6%free C < 3%
18 Alkalies (Na2O & K2O) may cause some dificulties if the cement is used with certain types of reactive aggregates in making concrete. The alkalies in the form of alkaline hydroxides can react with the reactive silica of the aggregate & resulting in volume expansion after hardening. This process may take years.Na2O & K2O ≤ 0.6%
19 Insoluble Residue: is that fraction of cement which is insoluble in HCl. It comes mainly from the silica which has not reacted to form compounds during the burning process in the kiln. All compounds of P.C. is soluble in HCl except the silica.The amount of I.R., determined by chemical analysis, serves to indicate the completeness of the reactions in the kiln.ASTM C 150 → I.R. ≤ 0.75%
20 Loss on Ignition (L.O.I.): is the loss in weight of cement after being heated to 1000°C. It indicates the prehydration or carbonation due to prolonged or improper storage of cement & clinker.If cement is exposed to air, water & CO2 are absorbed & by heating the cement upto 1000°C loose these two substances.ASTM C 150 → L.O.I. ≤ 3% for O.P.C.
21 COMPOUND COMPOSITION OF P.C. (OR CLINKER) Oxides interact with eachother in the kiln to form more complex products (compounds). Basically, the major compounds of P.C. can be listed as:NameChemical FormulaAbbreviationsTri Calcium Silicate3CaO.SiO2C3SDi Calcium Silicate2CaO.SiO2C2STri Calcium Aluminate3CaO.Al2O3C3ATetra Calcium Alumino Ferrite4CaO.Al2O3.Fe2O3C4AF
22 The degree to which the potential reactions can proceed to “equilibrium” depends on: Fineness of raw materials & their intermixing.The temperature & time that mix is held in the critical zone of the kiln.The grade of cooling of clinker may also be effective on the internal structure of major compounds.
23 There are also some minor compounds which constitute few %, so they are usually negligible. Moreover, portland cement compounds are rarely pure.For example in C3S, MgO & Al2O3 replaces CaO randomly.C3S→ALITE & C2S→BELITEFerrite Phase: C4AF is not a true compound. The ferrite phase ranges from C2AF to C6AF. *C4AF represents an average.
24 Methods of Determining Compound Composition Each grain of cement consists of an intimate mixture of these compounds.They can be determined by:MicroscopyX-Ray DiffractionBut due to the variabilities involved the compound composition is usually calculated using the oxide proportions.Calculations (Bouge’s Equations)
25 AssumptionsThe chemical reactions in the kiln proceeded to equilibrium.Compounds are in pure form such as C3S & C2SPresence of minor compounds are ignored.Ferrite phase can be calculated as C4AFAll oxides in the kiln have taken part in forming the compounds.
27 Ex:Given the following oxide composition of a portland cement clinker. CaO=64.9% SiO2=22.2%Al2O3=5.8% Fe2O3=3.1% MgO=4%Using Bogue’s eqn’s calculate the compound composition of the P.C. clinker?C3S=4.071* * * *3.1=52.1%C2S=2.876* *52.1=24.5%C3A=2.65* *3.1=10.1%
28 C4AF=3.043*3.1=9.4%To see the effect of change in oxide composition on the change in compound composition, assume that CaO is 63.9% & SiO2 is 23.2% and others are the same.C3S=40.4% , C2S=36.2% , C3A=10% , C4AF=9.4%C3S changed from 52.1%→40.4%C2S changed from 24.5%→36.2%1% change in CaO & SiO2 resulted in more than 10% change in C3S & C2S content.
29 Influence of Compound Composition on Characteristics of P.C. P.C.+water→the compounds in the cement undergo chemical reactions with the water independently, and different products result from these reactions.C3SC2SC3AC4AFRate of ReactionModerateSlowFastHeat LiberationHighLowVery HighEarly Cementitious ValueGoodPoorUltimate Cementitious Value
30 Average Compound Composition ASTM Type & Name of P.C.Average Compound CompositionC3SC2SC3AC4AFType I - O.P.C.4925128General PurposeType II - Modified46296For Moderate Heat of HydrationType III - High Early Strength5615C3S&C3A increased, C2S decreasedType IV - Low Heat P.C.30513C2S increasedType V - Sulfate Resistant P.C.43364Limit on C3A≤5%, 2C3A+C4AF≤25%
31 Hydration of P.C. Hydration: Chemical reactions with water. As water comes into contact with cement particles, hydration reactions immediately starts at the surface of the particles. Although simple hydrates such as C-H are formed, process of hydration is a complex one and results in reorganization of the constituents of original compounds to form new hydrated compounds.
33 At any stage of hydration the hardened cement paste (hcp) consists of: Hydrates of various compounds referred to collectively as GEL.Crystals of calcium hydroxide (CH).Some minor compound hydrates.Unhydrated cementThe residual of water filled spaces – pores.
34 As the hydration proceeds the deposits of hydrated products on the original cement grains makes the diffusion of water to unhydrated nucleus more & more difficult. Thus, the rate of hydration decreases with time & as a result hydration may take several years.Major compounds start to produce:Calcium-silicate-hydrate gelsCalcium hydroxide cementCalcium-alumino-sulfohydrates gel
35 At the beginning of mixing, the paste has a structure which consists of cement particles with water-filled space between them. As hydration proceeds, the gels are formed & they occupy some of this space.1cc of cement → 2.1cc of gelGel Pores: 28% of the total gel volume have diameter of μm. (very small-loss or gain of water is difficult)
36 Capillary Pores: 12.5 μm diameter, with varying sizes, shapes & randomly distributed in the paste. Volume of capillary pores decreases as hydration takes place. Water in capillary pores is mobile, can not be lost by evaporation or water can get into the pores. They are mainly responsible for permeability.- w/c ratiocapillary porosity- degree of hydration
37 C2S & C3S: 70-80% of cement is composed of these two compounds & most of the strength giving properties of cement is controlled by these compounds.Upon hydration both calcium-silicates result in the same products.2C3S+6H → C3S2H3 + 3CH2C2S+4H → C3S2H3 + CHCalcium-Silicate-Hydrate (C-S-H gel) is similar to a mineral called “TOBERMORITE”. As a result it is named as “TOBERMORITE GEL”
38 Upon hydration C3S & C2S, CH also forms which becomes an integral part of hydration products. CH does not contribute very much to the strength of portland cement.C3S having a faster rate of reaction accompanied by greater heat generation developes early strength of the paste. On the other hand, C2S hydrates & hardens slowly so results in less heat generation & developes most of the ultimate strength.
39 Higher C3S→higher early strength-higher heat generation (roads, cold environments) Higher C2S→lower early strength-lower heat generation (dams)C3A: is characteristically fast reacting with water & may lead to a rapid stiffening of the paste with a large amount of the heat generation (Flash-Set)-(Quick-Set). In order to prevent this rapid reaction gypsum is added to the clinker. Gypsum, C3A&water react to form relatively insoluble Calcium-Sulfo-Aluminates.
40 C3A+3CŚH2+26H→C6AŚ3H32 (calcium-alumino-trisulfohydrate “ettringite”) C3A+CŚH2+10H→C4AŚH12 (calcium- alumino-monosulfohydrate)C3A+3CŚH2+26H→C6AŚ3H32 (calcium-alumino-trisulfohydrate “ettringite”)When there is enough gypsum “ettringite” forms with great expansionIf there is no gypsum→flash-setmore gypsum→ettringiteformation increaseswhich will cause cracking
41 Also Calcium-Sulfo Aluminates are prone (less resistant) to sulfate attack & does not contribute much for strength. The cement to be used in making concretes that are going to be exposed to soils or waters that contain sulfates should not contain more than 5% C3A.C4AF: The hydration of ferrite phase is not well understand. Ferrite phase has lesser role in development of strength. The hydration products are similar to C3A. Alumina & iron oxide occur interchangebly in the hydration products.C4AŚH12 or C4FŚH12C6AŚ3H32 or C6FŚ3H32
42 HEAT OF HYDRATIONHydration process of cement is accompanied by heat generation (exothermic).As concrete is a fair insulator, the generated heat in mass concrete may result in expansion & cracking. This could be overcome by using suitable cement type.It could also be advantages for cold wheather concreting.The heat of hydration of OPC is on the order of cal/gr.About 50% of this heat is liberatedwithin 1-3 days & 75% within 7 days.By limiting C3S&C3A content heat of hydration can be reduced.
44 Heat of Hydration of Pure Compounds Heat of Hydration (cal/gr)C3S120C2S62C3A207C4AF100The amount of heat liberated is affected by the fractions of the compounds of the cement.Heat of Hydration(cal/gr)=120*(%C3S)+62*(%C2S)+207*(%C3A)+100*(C4AF)
46 FINENESS OF CEMENTAs hydration takes place at the surface of the cement particles, it is the surface area of cement particles which provide the material available for hydration. The rate of hydration is controlled by fineness of cement. For a rapid rate of hydration a higher fineness is necessary.
47 However,Higher fineness requires higher grinding (cost )Finer cements deteriorate faster upon exposure to atmosphere.Finer cements are very sensitive to alkali-aggregate reaction.Finer cements require more gypsum for proper hydration.Finer cements require more water.
48 Fineness of cement is determined by air permeability methods Fineness of cement is determined by air permeability methods. For example, in the Blaine air permeability method a known volume of air is passed through cement. The time is recorded and the specific surface is calculated by a formula.Fineness is expressed in terms of specific surface of the cement (cm2/gr). For OPC specific surface is cm2/gr.
50 SETTINGSetting refers to a change from liquid state to solid state. Although, during setting cement paste acquires some strength, setting is different from hardening.The water content has a marked effect on the time of setting. In acceptance tests for cement, the water content is regulated by bringing the paste to a standard condition of wetness. This is called “normal consistency”.
51 Normal consistency of O.P.C. Ranges from 20-30% by weight of cement. Vicat apparatus is used to determine normal consistency. Normal consistency is that condition for which the penetration of a standard weighed plunger into the paste is 10mm in 30sec. By trial & error determine the w/c ratio.In practice, the terms initial set&final set are used to describe arbitrary chosen time of setting. Initial set indicates the beginning of a noticeable stiffening & final set may be regarded as the start of hardening (or complete loss of plasticity).
53 Setting can be obtained by using the vicat apparatus. Initial setting time>45minASTM C150Final setting time<375minInitial > 1hr (60min)TS 19Final < 8hr (480min)
54 Factors Affecting Setting Time Temperature & HumidityAmount of WaterChemical Composition of CementFineness of Cement (finer cement, faster setting)Flash-setAbnormal SettingsFalse-set
55 Flash-Set: is the immediate stiffening of cement paste in a few minutes after mixing with water. It is accompanied by large amount of heat generation upon reaction of C3A with water.Gypsum is placed in cement to prevent flash-set. The rigidity can not be overcome & plasticity may not be regained without addition of water.Amount of gypsum must be such that it will be used upto almost hardening. Because expansion caused by ettringite can be distributed to the paste before hardening. More gypsum will cause undesirable expansion after hardening.
56 False-Set: is a rapid development of rigidity of cement paste without generation of much heat. This rigidity can be overcome & plasticity can be regained by further mixing without addition of water. In this way cement paste restores its plasticity & sets in a normal manner without any loss of strength.Probable Causes of False-Set:When gypsum is ground by too hot of a clinker, gypsum may be dehydrated into hemihydrate (CaSO4.1/2H2O) or anhydrate (CaSO4). These materials when react with water gypsum is formed, which results in stiffening of the paste.
57 Alkali oxides in cement may carbonate during storage Alkali oxides in cement may carbonate during storage. Upon mixing such a cement with water, these alkali carbonates will react with Ca(OH2) (CH-Calcium Hydroxide) liberated by hydrolysis of C3S resulting in CaCO3. CaCO3 precipates in the mix & results in false-set.
58 SOUNDNESS OF CEMENTSoundness is defined as the volume stability of cement paste.The cement paste should not undergo large changes in volume after it has set. Free CaO&MgO may result in unsound cement. Upon hydration C&M will form CH&MH with volume increase thus cracking.Since unsoundness is not apparent until several months or years, it is necessary to provide an accelerated method for its determination.Lechatelier Method: Only free CaO can be determined.Autoclave Method: Both free CaO&MgO can be determined.
59 STRENGTH OF CEMENTStrength tests are not carried out on neat cement pastes, because it is very difficult to form these pastes due to cohesive property of cement.Strength tests are carried out on cement mortar prepared by standard gradation (1 part cement+3 parts sand+1/2 part water)
60 Direct Tension (Tensile Strength): PP1”1”σt=P/1in2Difficult test procedure
66 TYPES OF PORTLAND CEMENT Cements of different chemical composition & physical characteristics may exhibit different properties when hydrated. It should thus be possible to select mixtures of raw materials for the production of cements with various properties.In fact several cement types are available and most of them have been developed to ensure durability and strength properties to concrete.
67 It should also be mentioned that obtaining some special properties of cement may lead to undesirable properties in another respect. For this reason a balance of requirements may be necessary and economic aspects should be considered.Standard Types: these cements comply with the definition of P.C., and are produced by adjusting the proportions of four major compounds.Special Types: these do not necessarily couply with the definiton of P.C. & are produced by using additional raw materials.
68 Standard Cements (ASTM) Type I: Ordinary Portland CementSuitable to be used in general concrete construction when special properties are not required.Type II: Modified Portland CementSuitable to be used in general concrete construction. Main difference between Type I&II is the moderate sulfate resistance of Type II cement due to relatively low C3A content (≤%8). Since C3A is limited rate of reactions is slower and as a result heat of hydration at early ages is less. *It is suitable to be used in small scale mass concrete like retaining walls.
69 Type III: High Early Strength P.C. Strength development is rapid.3 days f’c=7 days f’c of Type IIt is useful for repair works, cold weather & for early demolding.Its early strength is due to higher C3S & C3A content.Type IV: Low Heat P.C.Generates less heat during hydration & therefore gain of strengthis slower.In standards a maximum value of C3S&C3A& a minimum value for C2S are placed.It is used in mass-concrete and hot-weather concreting.
70 Type V: Sulfate Resistant P.C. Used in construction where concrete will be subjected to external sulfate attack – chemical plants, marine & harbor structures.During hydration C3A reacts with gypsum & water to form ettringite. In hardened cement paste calcium-alumino-hydrate can react with calcium&alumino sulfates, from external sources, to form ettringite which causes expansion & cracking.C-H and sulfates can react & form gypsum which again causes expansion & cracking.* In Type V C3A is limited to 5%.
71 Type IA, IIA, IIIA: Air Entrained Portland Cement Only difference is adding an air-entraining agent to the cement during manufacturing to increase freeze-thaw resistance by providing small sized air bubbles in concrete.
72 SPECIAL CEMENTS Portland Pozzolan Cement (P.P.C.) By grinding & blending P.C. Clinker+Pozzolan+GypsumP.P.C. Produces less heat of hydration & offers higher sulfate resistance so it can be used in marine structures & mass concrete.However, most pozzolans do not contribute to strength at early ages.The early strength of PPC is less.
73 Portland Blast Furnace Slag Cement (P.B.F.S.C.) By intergrinding B.F.S.+P.C. Clinker+GypsumThis cement is less reactive (rate of gain of strength & early strength is less but ultimate strength is same)High sulfate resistanceSuitable to use in mass concrete constructionUnsuitable for cold weather concretingBoth P.P.C.&P.B.F.S.C. Are called blended cements. Their heat of hydration & strength development are low in early days. Because upon adding water C3S compounds start to produce C-S-Hgels & CH. The Ch & the pozzolanic material react together to produce new C-S-H gels. That’s why the early strength is low but the ultimate strength is the same when compared to O.P.C.
74 White Portland CementW.P.C. İs made from materials containing a little iron oxide & manganese oxide.Fe2O3 + MnO ≤ 0.8%To avoid contamination by coal ash, oil is used as fuel.To avoid contamination by iron during grinding, instead of steel balls nickel-molybdenum alloys are used.
75 High Alumina CementThe raw materials for H.A.C. İs limestone and Bauxite (Al2O3 & Fe2O3)These raw materials are interground & introduced in the kiln clinkered at 1600°C. Then the obtained material is ground to a fineness of cm2/gr.The oxide composition is quite differentAl2O3 → 40-45%CaO → 35-42%Fe2O3 → 5-15%SiO2 → 4-10%
76 Major compounds are CA & C2S It is basically different from O.P.C. & the concrete made from this cement has very different properties.It has high sulfate resistance.Very high early strength (emergency repairs)About 80% of ultimate strength is obtained within 24 hours. But the strength is adversely affected by temperature. The setting time is not as rapid as gain of strength.Initial setting time is 4 hrs & final setting time is 5 hrs.
77 STANDARD TURKISH CEMENTS (TS 19) – Cancelled TS 19 groups them into 3P.Ç → min. Compressive strength is 32.5 MPa in 28 days.P.Ç. 42.5P.Ç. 52.5Special Cements are:TS 20 –Blast Furnace Slag CementCÇ 32.5 – Cüruflu ÇimentoCÇ 42.5TS 21 – White Portland Cement BPÇTS22 – Masonry Cement, HÇ 16 (Harç Çimentosu)TS 26 – Trass Cement, TÇ 32.5 (Traslı Çimento)TS 640 – Fly Ash Cement, UKÇ 32.5 (Uçucu Küllü Çimento)
78 TS EN 197-1 NEW 27 different cements CEM cements CEM I – Portland CementCEM II – Portland Composite CementCEM III – Portland Blast Furnace Slag CementCEM IV – Pozzolanic CementCEM V – Composite Cement27 different cements
79 TS EN 197-1 CEM cements : Clinker, major and minor mineral admixtures Binding property is mainly due to hydration of calcium-silicatesReactive C + Reactive S > 50%Clinker, major and minor mineral admixturesClinker + Major + Minor = 100% (mass) + GypsumMajor > 5% by massMinor 5% by mass
80 TS EN 197-1 Mineral Admixtures K : ClinkerD : Silica FumeP : Natural PozzolanQ : Calcined Natural PozzolanT : Calcined ShaleW : Class – C Fly AshV : Class – F Fly AshL : Limestone (Organic compound < 0.5%)LL : Limestone (Organic compound < 0.2%)S : Granulated Blast Furnace Slag
81 TS EN 197-1 Composition A : Lowest amount of mineral admixture B : Mineral admixture amount is > AC : Mineral admixture amount is > B
82 TS EN CompositionCEM I : Portland Cement95-100% K + 0-5% Minor
83 TS EN 197-1 Composition CEM II : Portland Composite Cement CEM II/A-S : Portland Slag Cement80-94% K % S + 0-5% MinorCEM II/B-S : Portland Slag Cement65-79% K % S + 0-5% MinorCEM II/B-P : Portland Pozzolanic Cement65-79% K % P + 0-5% MinorCEM II/A-V : Portland Fly Ash Cement80-94% K % V + 0-5% Minor
84 TS EN 197-1 Composition CEM III : Portland Blast Furnace Slag Cement CEM III/A : Portland Blast Furnace Slag Cement35-64% K % S + 0-5% MinorCEM III/B : Portland Blast Furnace Slag Cement20-34% K % S + 0-5% MinorCEM III/C : Portland Blast Furnace Slag Cement5-19% K % S + 0-5% Minor
85 TS EN 197-1 Composition CEM IV : Pozzolanic Cement CEM IV/A : Pozzolanic Cement65-89% K % (D,P,Q,V,W) + 0-5% MinorCEM IV/B : Pozzolanic Cement45-64% K % (D,P,Q,V,W) + 0-5% Minor
86 TS EN 197-1 Composition CEM V : Composite Cement CEM V/A : Composite Cement40-64% K % S % (P,Q,V) + 0-5% MinorCEM V/B : Composite Cement20-38% K % S % (P,Q,V) + 0-5% Minor